DOI: 10.17188/1299810
title: Materials Data on Li24Mn11CrO36 by Materials Project

description: Li24CrMn11O36 is beta Polonium-derived structured and crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twenty-four inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the second Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with two equivalent CrO6 octahedra, edges with four MnO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are four shorter (2.08 Å) and two longer (2.11 Å) Li–O bond lengths. In the third Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.21 Å. In the fourth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There are a spread of Li–O bond distances ranging from 2.02–2.18 Å. In the fifth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.21 Å. In the sixth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six MnO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are four shorter (2.08 Å) and two longer (2.10 Å) Li–O bond lengths. In the seventh Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–9°. There are a spread of Li–O bond distances ranging from 2.02–2.18 Å. In the eighth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the ninth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.05–2.21 Å. In the tenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six MnO6 octahedra. The corner-sharing octahedra tilt angles range from 8–9°. There are four shorter (2.08 Å) and two longer (2.10 Å) Li–O bond lengths. In the eleventh Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.03–2.19 Å. In the twelfth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, an edgeedge with one CrO6 octahedra, edges with three MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.05–2.21 Å. In the thirteenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the fourteenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are two shorter (2.03 Å) and four longer (2.17 Å) Li–O bond lengths. In the fifteenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, an edgeedge with one CrO6 octahedra, edges with five MnO6 octahedra, and edges with six LiO6 octahedra. The corner-sharing octahedral tilt angles are 9°. There are a spread of Li–O bond distances ranging from 2.07–2.10 Å. In the sixteenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the seventeenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.03–2.19 Å. In the eighteenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the nineteenth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one CrO6 octahedra, corners with two LiO6 octahedra, corners with three MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the twentieth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are two shorter (2.03 Å) and four longer (2.17 Å) Li–O bond lengths. In the twenty-first Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. In the twenty-second Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six MnO6 octahedra. The corner-sharing octahedral tilt angles are 9°. There are four shorter (2.08 Å) and two longer (2.10 Å) Li–O bond lengths. In the twenty-third Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six LiO6 octahedra, edges with six LiO6 octahedra, and edges with six MnO6 octahedra. The corner-sharing octahedral tilt angles are 9°. There are four shorter (2.08 Å) and two longer (2.10 Å) Li–O bond lengths. In the twenty-fourth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with two LiO6 octahedra, corners with four MnO6 octahedra, edges with four MnO6 octahedra, and edges with eight LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Li–O bond distances ranging from 2.06–2.20 Å. Cr6+ is bonded to six O2- atoms to form CrO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Cr–O bond distances ranging from 1.90–1.98 Å. There are eleven inequivalent Mn+3.82+ sites. In the first Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedral tilt angles are 7°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the second Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedral tilt angles are 7°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the third Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, an edgeedge with one MnO6 octahedra, edges with two equivalent CrO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 5–8°. There are a spread of Mn–O bond distances ranging from 1.92–1.95 Å. In the fourth Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the fifth Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedral tilt angles are 7°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the sixth Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedral tilt angles are 7°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the seventh Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedral tilt angles are 7°. There are a spread of Mn–O bond distances ranging from 1.93–1.95 Å. In the eighth Mn+3.82+ site, Mn+3.82+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six LiO6 octahedra, edges with three MnO6 octahedra, and edges with nine LiO6 octahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Mn–O b